Validation of the Resonalyser method: an inverse method for material identification


 Tyrone Walton
 1 years ago
 Views:
Transcription
1 Validation of the Resonalyser method: an inverse method for material identification T. Lauwagie, H. Sol,. Roebben 3, W. Heylen and Y. Shi Katholieke Universiteit Leuven (KUL) Department of Mechanical ngineering (PMA), Celestijnenlaan 300b, 300 Heverlee, Belgium Vrije Universiteit Brussel (VUB) Department Mechanics of Materials and Constructions (MMC) Pleinlaan, 050 Brussels, Belgium 3 Katholieke Universiteit Leuven (KUL) Department of Metallurgy and Materials ngineering (MTM) Kasteelpark Arenberg, 300 Heverlee, Belgium Abstract The Resonalyser method uses resonance frequencies measured on rectangular plate specimens to identify orthotropic material properties. An inverse technique is used to update the material properties in a numerical model of the test plate. The obtained material properties of steel and aluminum test plates are validated with the results of standard impulse excitation tests and standard tensile tests. Impulse excitation tests (IT) were performed on beam specimens cut in different material directions of the plates. IT uses inplane and torsional vibration modes to identify the Young s moduli, shear moduli and Poisson s ratios in the orthotropic material axes and offaxis directions. It was found that the obtained results were situated well within the error intervals of the tensile test results and that the results from IT were in good agreement with the Resonalyser results. The error bounds of the Resonalyser tests have the same small magnitude as impulse testing. Both methods based on vibration measurements are accurate and produce repeatable results. Introduction Many engineering materials behave in an anisotropic manner: their response to external solicitations depends on the loading direction. A simple but common form of anisotropy is orthotropy. The elastic behavior of materials having orthotropic symmetry axes (e.g. rolled metal sheets or longfiber reinforced composites), in a state of plane stress, can be described by the following relation between strains and stresses: ε = ν ε γ 0 ν 0 0 σ 0. σ τ () In relation (), {ε i } represents the strain components, {σ j } the stress components, i the Young's modulus in the idirection, ν ij the Poisson's ratios, and is the shear modulus in the (,) plane. If linear material behavior is assumed, the elastic properties i, ν ij and are also called the 'engineering constants'. Due to the symmetry of the compliance matrix in (), only four (instead of five) independent engineering constants occur: e.g.,, ν and. Knowledge of the elastic properties of materials is important for their use in structural applications, as well as for the improvement of the processes used to transform them into components. lastic properties also play a major role in the vibration behavior of constructions. This observation can be inverted, leading to the conclusion that the vibration behavior of samples of a particular material can be used to determine the material s elastic properties. 687
2 688 PROCDINS OF ISMA00  VOLUM II The Impulse xcitation Technique (IT) is based on this observation. IT uses analytical formulas to calculate the elastic moduli from the resonance frequencies of a test beam, and serves as an alternative to the more traditional static tests in which a controlled load (or deformation) is applied while monitoring the resulting deformation (or load). Both IT and static tests (e.g. tensile tests) are standardprocedures for assessing the stiffness of an elongated test sample along its long axis (IT: NV83 and ASTM 876, tensile tests: ). More recently, an inverse method, called "Resonalyser procedure", was developed to determine all four engineering constants for orthotropic materials from the resonance frequencies of rectangular plate samples []. In this paper, standard tensile and IT tests are used to validate the accuracy and sensitivity of the Resonalyser procedure for the case of rolled metal sheets. []. This name has been chosen based on the observation that the frequencies of the anticlastic and synclastic modes (figure ) are particularly sensitive for changes of the Poisson's ratio of the plate material. A (hypothetical) material with a zero value for Poisson's ratio would make the frequencies of the anticlastic and synclastic mode coincide. Figure gives an overview of the five first mode shapes of a Poisson test plate. The mode shapes of the first three resonances (the torsional, anticlastic and synclastic modes) will always appear in this fixed sequence. The th and 5th frequencies coincide for a perfect Poisson plate. Due to inevitable small imperfections the order of the fourth and fifth mode, an orthogonal couple of torsionbending mode shapes, can not be predicted a priori, and will have to be determined during the experiment. Theoretical background. The Poisson test plate The Resonalyser procedure is a mixed numericalexperimental method that aims to identify the engineering constants of orthotropic materials using measured resonance frequencies of freely suspended rectangular plates. Using rectangular plates as test specimen allows the simultaneous identification of,, v and. In addition, the obtained elastic material properties are homogenised over the plate surface and hence suitable as input values for finite element models of structures. Also the amount of machining induced edge damage is reduced when using plate shaped rather than elongated specimens. The basic principle of the Resonalyser is to compare experimentally measured frequencies with the numerically computed frequencies of a finite element model of the test plate. Such an inverse procedure can only yield good results if the numerical model is controllable and if the elastic properties can be observed through the measured data [3]. This requires that in the selected series of frequencies at least one of the frequencies varies significantly for variations of each of the elastic properties. It can be shown that this requirement is fulfilled if the length to width ratio of the test plate Length approximately complies with = Width. A plate with such a ratio is called a 'Poisson test plate' Torsional Anticlastic Synclastic TorBenX TorBenY Figure : The first 5 mode shapes of a Poisson test plate.. Identification of the engineering constants A detailed scheme of the Resonalyser procedure is given in figure. Starting with estimated initial values, the engineering constants in a finite element model of the test plate are iteratively updated until the first five computed resonance frequencies match the measured frequencies. In the finite element model, the plate dimensions and mass are considered as known quantities and thus fixed values. The four engineering constants are stored in the parameter column {p}. The updating of {p} is realized by minimizing a cost function C(p): C( p ) = T ( { f f ( p )} [ W f ) exp FM ]{ f exp f FM ( p )} ( 0 ) T ( ) ( 0 ) { p p} [ W ]{ p p} p in which C(p) is a NP cost function yielding a scalar value, NP= is the number of ()
3 MATRIAL CHARACTRISATION BASD ON DYNAMIC MASURMNTS 689 Starting values for the material properties:,, and ν. Plate geometry Plate mass Test specimen Finite lement Model xperimental Modal Analysis Frequency sensitivities Numerical  resonance frequencies  mode shapes xperimental  resonance frequencies  mode shape order Mode pairs Frequency differences Material property corrections Improved material properties No Material property corrections < precision Yes Identified material properties Figure : Detailed flowchart of the Resonalyser procedure: material identification by comparing the experimentally measured and computed resonance frequencies of a test plate.
4 690 PROCDINS OF ISMA00  VOLUM II material parameters:,, ν and, {p (0) } is a (NP ) vector and contains the initial estimates for the material parameters, {f FM (p)} is a (NF ) output column containing the NF=5 computed frequencies using parameter values {p}, {f exp } contains the (NF ) measured frequencies, [W (f) ] is a (NF NF) weighting matrix applied on the difference between the measured and the calculated frequency column, [W (p) ] is a (NP NP) weighting matrix for the difference between the initial parameter column {p (0) } and the parameter column {p}. The cost function C(p) has a minimal value for the optimal parameter values column {p (opt) }. The value of this {p (opt) } can be made independent on the choice of the weighting matrices [W (f) ] and [W (p) ] in the cost function. The choice and role of [W (f) ] and [W (p) ] is discussed, among others, in [], [5] and [6]. The updating of the initial parameter column toward {p (opt) } by minimization of the cost function is given by the following recurrence formula in iteration step (j): ( j ) ( ) ( p ) ( ) ( f ) ( ) { p } = { p } [ W S W S ] j j T j S ( j ) W ( f ) ( ) { f f ( p )} j exp fem (3) In (3) S is the sensitivity matrix containing the partial derivatives of the numerical frequencies with respect to the elements of the parameter column. The numerical model of the test plate is based on the LoveKirchhoff theory [7]. The applicability of this theory is mainly limited by the thickness of the plate. Traditionally, plates with a length/thickness ratio that exceeds a factor of 50 are considered as sufficiently thin. The tested materials and applied vibration amplitudes, do not violate additional assumptions made by the LoveKirchhoff theory. Very accurate eight order polynomial Lagrange functions are taken as shape functions in the used numerical finite element model of the test plate []. The stiffness matrix of the test plate is evaluated in each iteration cycle using standard finite element procedures with the values of the parameter column {p} at that moment [8]. The computed resonance frequencies are obtained by solving a generalized eigenvalue problem composed with the constant mass matrix and the evaluated stiffness matrix [8]. The iteration procedure ends if convergence of {p} is reached. The values of the engineering constants in {p} after the last iteration cycle are considered as the result of the Resonalyser procedure. The whole identification procedure takes typically less than 5 seconds on a standard pentiumiii PC. 3 Material Identification 3. Test specimen selection and preparation Commercially available 608 Alalloy, 30 stainless steel, and CuZn37 brassplates were obtained in the hotrolled state. The 30 stainless steel is an austenitic steel with as main alloying elements chromium (8.5 %) and Ni (8.5 %). The plate used in this investigation has a thickness of 6 mm. The 608 aluminium alloy contains as main alloying elements silicon (0.7.3 %), iron (0.5 %), Mn (0..0 %) and Mg (0.6. %). The plate used in this investigation has a thickness of 5 mm. The tested brass is a Cu (6 6 %), Zn (35 37 %) alloy and contains Ni (0. 3 %), Fe (0. %), and Sn (0. %) as main alloying elements. The used plate had a nominal thickness of 5 mm. Tensile, Resonalyser and/or IT test samples were produced from single plates of each material. Relatively large samples were cut and carefully machined (to within / mm) to eliminate or at least reduce the effect of inaccurate sample dimensions on the calculated material properties. The thickness of the samples was not changed: the rolling surfaces were left untouched. The standard deviation of the thickness was 0.03 mm. IT and tensile tests were performed on samples cut along the rolling direction and at the following angles:  90, 60, 5, 30, 30, 5, 60 and 90. Plates for the Resonalyser tests had sides parallel to and at 90 with the rolling direction. 3. Standard mechanical tests The elastic moduli were determined following standard IT and tensile test procedures. IT is based on the measurement of the fundamental flexure and torsion resonance frequencies of slender beam samples. Analytical equations, based on elastic beam theory, relate these frequencies to the Young s and shear modulus while assuming isotropic material behaviour. ITtests were performed on rectangular beamlike samples of nominal size mm for the aluminium, mm for the brass, and mm for the steel, using the RFDA apparatus (IMC nv, Diepenbeek, Belgium) described in [9], following the guidelines provided by ASTM and NV83.
5 MATRIAL CHARACTRISATION BASD ON DYNAMIC MASURMNTS 69 Tensile tests were performed on flat dogbone shaped samples of length 00 mm, 65 mm gauge length and gauge section of 63 mm for the aluminium and 73 mm for the steel samples. The strain was determined in a first instance using a clipon extensometer (gauge length 50 mm). Afterwards, tensile tests were repeated on the same samples, now using biaxial strain gauges, in order to identify Poisson s ratio. For each test, the load was applied and removed periodically, with an increasing amplitude (3, 6 and 9 kn for the aluminum samples, and, and 6 kn for the steel samples). xperimental Results. Impulse xcitation Test The Young s modulus was calculated from the fundamental in plane bending frequency (IP Bending). The shear modulus was calculated from the fundamental torsion frequency of the beam. Figure 3 and show the obtained material properties for different orientations of the test beams.. Uniaxial tensile tests The Poisson s ratios were identified by means of biaxial strain gauges, while the measurement of the Young s moduli was performed with a clipon extensometer. The values of the elastic moduli were derived from the stressstrain curves obtained during the loading phase of the test cycle. The measured material properties are plotted in figure 3 and..3 Resonalyser tests The material properties were obtained with the procedure described in paragraph. Table and table compare the measured resonance frequencies with the analytical frequencies of the Resonalyser s Fmodel. Freq. xp. Freq. Num. Difference Mode % Mode % Mode % Mode % Mode % Table : The obtained frequency match and material properties for the aluminum plate. Freq. xp. Freq. Num. Difference Mode % Mode % Mode % Mode % Mode % Table : The obtained frequency match and material properties for the steel plate. The Resonalyser method only identifies directly material properties in the direction of the main axes. The offaxis elastic properties of an orthotropic material can be calculated with the following equations [0]: x = cos θ ( sin θ cos θ ) ν sin θ cos θ sin θ ν ν = xy x sin θ cos θ y xy = = sin θ ν ( sin θ cos θ ) ν sin θ cos θ sin θ cos θ.. Comparison of the results cos θ As opposed to the Resonalyser results, the offaxis properties identified with IT and tensile tests are directly measured. Figures 3 and compare these results with the curves obtained from formula () and the Resonalyser procedure. 5 Discussion The anisotropy of the aluminum material is clearly more pronounced (about % difference between minimum and maximum Young s modulus) than that of the investigated stainless steel (less than %). 5. Correlation between the results of the different tests For both the aluminum and steel material a good correlation between the results of the Young s moduli in the two main directions obtained with the three different methods is found. However, in the case of the aluminum plate, the Resonalyser procedure results in lower offaxis elastic moduli ()
6 69 PROCDINS OF ISMA00  VOLUM II (Pa) 7 70 (Pa) Resonalyser IT (IP) Tensile Tests Resonalyser IT (Tors) ν () Resonalyser IT (IP) Tensile Tests Figure 3: Comparison of the results of the three different methods for the modulus, modulus and Poisson s ratio ν for aluminum. (Pa) (Pa) Resonalyser IT (IP) Tensile Tests 0.3 Resonalyser IT (Tors) 0.3 ν () Resonalyser IT (IP) Tensile Tests Figure : Comparison of the results of the three different methods for the modulus, modulus and Poisson s ratio ν for steel.
7 MATRIAL CHARACTRISATION BASD ON DYNAMIC MASURMNTS 693 than IT. The tensile tests performed on the specimen in the ±5 directions yielded values that were situated between the results of the two dynamic test methods. The spreading on the results of the tensile tests was too high to indicate if IT overestimated or if the Resonalyser method underestimated the offaxis elastic moduli. The steel material was too isotropic to compare the difference between the correlation of the onaxis and offaxis Young s moduli. For both the aluminum and steel material the values of shear modulus obtained with IT are higher than the values obtained with the Resonalyser method, but there is a good correlation between the values of the shear moduli in the ±5 directions. The comparison between the Poisson s ratios obtained with IT and Resonalyser reveals a complete lack of agreement between the results of these two methods. However, the tensile tests and the Resonalyser procedure reveal the same directional dependency of Poisson s ratio, for the aluminum. IT fails to identify Poisson s ratio for orthotropic materials, since the IT identificationprocedure is based on a relation between Poisson s ratio and the elastic and shear modulus, which only holds for fully isotropic materials. 5. Verification To verify whether the observed differences of the Young s moduli in the offaxis directions and shear moduli in the onaxis directions are specifically related to the used aluminum material, rather than a more general problem, the Resonalyser method and IT were used to identify the properties of the brass material. Three IT beams in the 0, 5 and 90 directions and one Resonalyser plate ( mm) were machined. The brass samples were tested in the same way as the aluminum and steel samples. (Pa) Resonalyser IT (IP) Figure 5: Comparison of the Young s moduli obtained with the Resonalyser and IT for the brass material. The obtained Young s moduli are presented in figure 5. Once again, a good correlation between the onaxis properties is found. As for the aluminum, the Young s moduli found by IT are higher than those found by the Resonalyser procedure. Like in the previous tests, the shear modulus in the zero direction obtained with IT exceeds the shear modulus obtained with the Resonalyser method, figure 6. (Pa) Resonalyser Figure 6: Comparison of the shear moduli obtained with the Resonalyser and IT for the brass material. IT 5.3 The influence of warping The Kirchhoff plate theory, used in the Resonalyser s Fmodel, assumes that a plane perpendicular to the central plane of the plate before deformation, remains flat and perpendicular to the central plane after deformation. The Kirchhoff thin plate theory does not account for warping deformations caused by shear stresses induced by torsion. For a given set of material properties, this could lead to an overestimation of the resonance frequency of all the torsion modes. The Resonalyser procedure will compensate this effect by artificially reducing the shear modulus. This is exactly what is observed when comparing the IT and Resonalyser results. This could explain why the shear modulus found with the Resonalyser is lower that the shear modulus found with IT. An increase of the shear modulus will also lead to an increase of the offaxis elastic properties calculated with (). Further research will be needed to confirm whether warping deformation is really causing the observed differences between the results of the two dynamic measurement methods.
8 69 PROCDINS OF ISMA00  VOLUM II 6 Conclusion In this paper three methods for measuring the elastic properties of plate materials are shown to quantify the degree of elastic anisotropy of aluminum and stainless steel sheets. The results obtained with different techniques (uniaxial tension, impulse excitation technique and a mixednumericalexperimental technique) confirm each other. Small differences between the offaxis elastic moduli obtained with the Resonalyser and IT technique were observed. The influence of warping is proposed as an explanation for these differences. Further research is needed to prove the validity of this theory. [7] Love, A..H., Mathematical theory of elasticity (th edition), Cambridge University Press, 97. [8] Zienkiewicz, O.C., The finite element method (3rd edition), Mc.raw Hill, 977. [9] Roebben,., Bollen, B., Brebels, A., Van Humbeeck, J. and Van der Biest, O., Impulse excitation apparatus to measure resonant frequencies, elastic moduli and internal friction at room and high temperature, Rev. Sci. Instr., 997, 68, 5. [0] Jones, R. M., Mechanics of composite materials, MacrawHill, USA, 975. Acknowledgements This work was performed in the framework of the RAMATIC research project supported by the Flemish Institute for the Promotion of Scientific and Technological Research in Industry IWT. ert Roebben is a postdoctoral fellow of the FWO Vlaanderen. References (style: Reference) [] Sol, H. & Oomens, C., Material Identification Using Mixed Numerical xperimental Methods, Kluwer Academic Publishers, 997. [] Hua, H., Identification of Plate Rigidities of Anisotropic Rectangular Plates, Sandwich Panels and Orthotropic Circular Disks using Vibration Data, Ph.D. Thesis presented at the Vrije Universiteit Brussel, Belgium, 993. [3] Kreindler,., Sarachik, P..,. On the concepts of Controllability and Observability of linear Systems, I trans., A.C., Vol. AC9, 96. [] Sol, H., Identification of anisotropic plate rigidities using free vibration data, Ph.D.Thesis presented at the Vrije Universiteit Brussel, Belgium,986. [5] Collins, J.D., Hart,.C., Hasselman, T.K., Kennedy, B., Statistical Identification of Structures, AIAA Journal, (), pp.8590, 97. [6] Sol, H. et all., La procedure Resonalyser, La revue des laboratoires d'ssais, n 6, pp.0, 996.
IDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE
IDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE Hugo Sol, hugos@vub.ac.be Massimo Bottiglieri, Massimo.Bottiglieri@vub.ac.be Department Mechanics of Materials
More informationComparison of different identification techniques for measurement of quasizero Poisson s ratio of fabricreinforced laminates
Composites: Part A 38 (2007) 2047 2054 www.elsevier.com/locate/compositesa Comparison of different identification techniques for measurement of quasizero Poisson s ratio of fabricreinforced laminates
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationSTANDARD SAMPLE. Reduced section " Diameter. Diameter. 2" Gauge length. Radius
MATERIAL PROPERTIES TENSILE MEASUREMENT F l l 0 A 0 F STANDARD SAMPLE Reduced section 2 " 1 4 0.505" Diameter 3 4 " Diameter 2" Gauge length 3 8 " Radius TYPICAL APPARATUS Load cell Extensometer Specimen
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationLab Exercise #5: Tension and Bending with Strain Gages
Lab Exercise #5: Tension and Bending with Strain Gages Prelab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationBE Semester I ( ) Question Bank (MECHANICS OF SOLIDS)
BE Semester I ( ) Question Bank (MECHANICS OF SOLIDS) All questions carry equal marks(10 marks) Q.1 (a) Write the SI units of following quantities and also mention whether it is scalar or vector: (i)
More informationStudy on the influence of design parameter variation on the dynamic behaviour of honeycomb sandwich panels
Study on the influence of design parameter variation on the dynamic behaviour of honeycomb sandwich panels Stijn Debruyne 2, Dirk Vandepitte 1, Eric Debrabandere 2, Marc Hongerloot 2 1 Department of Mechanical
More informationThe University of Melbourne Engineering Mechanics
The University of Melbourne 436291 Engineering Mechanics Tutorial Four Poisson s Ratio and Axial Loading Part A (Introductory) 1. (Problem 922 from Hibbeler  Statics and Mechanics of Materials) A short
More information2766. Differential quadrature method (DQM) for studying initial imperfection effects and pre and postbuckling vibration of plates
2766. Differential quadrature method (DQM) for studying initial imperfection effects and pre and postbuckling vibration of plates Hesam Makvandi 1, Shapour Moradi 2, Davood Poorveis 3, Kourosh Heidari
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationCOMPARISON OF THE TESTS CHOSEN FOR MATERIAL PARAMETER IDENTIFICATION TO PREDICT SINGLE POINT INCREMENTAL FORMING FORCES
International Deep Drawing Research Group IDDRG 28 International Conference 1618 June 28, Olofström, Sweden COMPARISON OF THE TESTS CHOSEN FOR MATERIAL PARAMETER IDENTIFICATION TO PREDICT SINGLE POINT
More informationME 207 Material Science I
ME 207 Material Science I Chapter 3 Properties in Tension and Compression Dr. İbrahim H. Yılmaz http://web.adanabtu.edu.tr/iyilmaz Automotive Engineering Adana Science and Technology University Introduction
More informationSome Aspects Of Dynamic Buckling of Plates Under In Plane Pulse Loading
Mechanics and Mechanical Engineering Vol. 12, No. 2 (2008) 135 146 c Technical University of Lodz Some Aspects Of Dynamic Buckling of Plates Under In Plane Pulse Loading Katarzyna Kowal Michalska, Rados
More informationSEMM Mechanics PhD Preliminary Exam Spring Consider a twodimensional rigid motion, whose displacement field is given by
SEMM Mechanics PhD Preliminary Exam Spring 2014 1. Consider a twodimensional rigid motion, whose displacement field is given by u(x) = [cos(β)x 1 + sin(β)x 2 X 1 ]e 1 + [ sin(β)x 1 + cos(β)x 2 X 2 ]e
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each.
GTE 2016 Q. 1 Q. 9 carry one mark each. D : SOLID MECHNICS Q.1 single degree of freedom vibrating system has mass of 5 kg, stiffness of 500 N/m and damping coefficient of 100 Ns/m. To make the system
More informationThe science of elasticity
The science of elasticity In 1676 Hooke realized that 1.Every kind of solid changes shape when a mechanical force acts on it. 2.It is this change of shape which enables the solid to supply the reaction
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationChapter 2: Elasticity
OHP 1 Mechanical Properties of Materials Chapter 2: lasticity Prof. Wenjea J. Tseng ( 曾文甲 ) Department of Materials ngineering National Chung Hsing University wenjea@dragon.nchu.edu.tw Reference: W.F.
More informationUnit 18 Other Issues In Buckling/Structural Instability
Unit 18 Other Issues In Buckling/Structural Instability Readings: Rivello Timoshenko Jones 14.3, 14.5, 14.6, 14.7 (read these at least, others at your leisure ) Ch. 15, Ch. 16 Theory of Elastic Stability
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationME 243. Mechanics of Solids
ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET Email: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil
More informationTensile stress strain curves for different materials. Shows in figure below
Tensile stress strain curves for different materials. Shows in figure below Furthermore, the modulus of elasticity of several materials effected by increasing temperature, as is shown in Figure Asst. Lecturer
More informationMAAE 2202 A. Come to the PASS workshop with your mock exam complete. During the workshop you can work with other students to review your work.
It is most beneficial to you to write this mock final exam UNDER EXAM CONDITIONS. This means: Complete the exam in 3 hours. Work on your own. Keep your textbook closed. Attempt every question. After the
More informationISHIK UNIVERSITY DEPARTMENT OF MECHATRONICS ENGINEERING
ISHIK UNIVERSITY DEPARTMENT OF MECHATRONICS ENGINEERING QUESTION BANK FOR THE MECHANICS OF MATERIALSI 1. A rod 150 cm long and of diameter 2.0 cm is subjected to an axial pull of 20 kn. If the modulus
More informationMassachusetts Institute of Technology Department of Aeronautics and Astronautics Cambridge, MA Problem Set 14
Massachusetts Institute of Technology Department of Aeronautics and Astronautics Cambridge, MA 02139 16.01/16.02 Unified Engineering I, II Fall 2003 Problem Set 14 Name: Due Date: 12/9/03 F18 F19 F20 M19
More informationWORKBOOK MECHANICS OF MATERIALS AND ELEMENTS OF ENGINEERING STRUCTURES
WORKBOOK MECHANICS OF MATERIALS AND ELEMENTS OF ENGINEERING STRUCTURES LUBLIN 014 Authors: Sylwester Samborski, Andrzej Teter and Marcin Bocheński Desktop publishing: Sylwester Samborski, Andrzej Teter
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationGATE SOLUTIONS E N G I N E E R I N G
GATE SOLUTIONS C I V I L E N G I N E E R I N G From (1987018) Office : F16, (Lower Basement), Katwaria Sarai, New Delhi110016 Phone : 01165064 Mobile : 81309090, 9711853908 Email: info@iesmasterpublications.com,
More informationPDDC 1 st Semester Civil Engineering Department Assignments of Mechanics of Solids [ ] Introduction, Fundamentals of Statics
Page1 PDDC 1 st Semester Civil Engineering Department Assignments of Mechanics of Solids [2910601] Introduction, Fundamentals of Statics 1. Differentiate between Scalar and Vector quantity. Write S.I.
More information8 Properties of Lamina
8 Properties of Lamina 8 ORTHOTROPIC LAMINA An orthotropic lamina is a sheet with unique and predictable properties and consists of an assemblage of fibers ling in the plane of the sheet and held in place
More informationNomenclature. Length of the panel between the supports. Width of the panel between the supports/ width of the beam
omenclature a b c f h Length of the panel between the supports Width of the panel between the supports/ width of the beam Sandwich beam/ panel core thickness Thickness of the panel face sheet Sandwich
More informationAn orthotropic damage model for crash simulation of composites
High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures
More informationLateraltorsional buckling of orthotropic rectangular section beams
ateraltorsional buckling of orthotropic rectangular section beams Summary Bambang SUYOAMONO Professor Department of Civil ngineering, Parahyangan Catholic University Bandung, Indonesia Adhijoso JONDO
More informationEvaluation of inplane orthotropic elastic constants of paper and paperboard
Evaluation of inplane orthotropic elastic constants of paper and paperboard T. Yokoyama and K. Nakai Department of Mechanical Engineering, Okayama University of Science  Ridaicho, Okayama 75, Japan
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationChapter 4 Analysis of a cantilever
Chapter 4 Analysis of a cantilever Before a complex structure is studied performing a seismic analysis, the behaviour of simpler ones should be fully understood. To achieve this knowledge we will start
More informationSolid Mechanics Chapter 1: Tension, Compression and Shear
Solid Mechanics Chapter 1: Tension, Compression and Shear Dr. Imran Latif Department of Civil and Environmental Engineering College of Engineering University of Nizwa (UoN) 1 Why do we study Mechanics
More informationSTRENGTH OF MATERIALSI. Unit1. Simple stresses and strains
STRENGTH OF MATERIALSI Unit1 Simple stresses and strains 1. What is the Principle of surveying 2. Define Magnetic, True & Arbitrary Meridians. 3. Mention different types of chains 4. Differentiate between
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationMassachusetts Institute of Technology Department of Aeronautics and Astronautics Cambridge, MA Problem Set 14
Massachusetts Institute of Technology Department of Aeronautics and Astronautics Cambridge, MA 02139 16.01/16.02 Unified Engineering I, II Fall 2003 Problem Set 14 Name: Due Date: 12/9/03 F18 F19 F20 M19
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown.
D : SOLID MECHANICS Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown. Q.2 Consider the forces of magnitude F acting on the sides of the regular hexagon having
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationStructural Dynamics Lecture Eleven: Dynamic Response of MDOF Systems: (Chapter 11) By: H. Ahmadian
Structural Dynamics Lecture Eleven: Dynamic Response of MDOF Systems: (Chapter 11) By: H. Ahmadian ahmadian@iust.ac.ir Dynamic Response of MDOF Systems: ModeSuperposition Method ModeSuperposition Method:
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationConstitutive Equations (Linear Elasticity)
Constitutive quations (Linear lasticity) quations that characterize the physical properties of the material of a system are called constitutive equations. It is possible to find the applied stresses knowing
More informationExperimental Study and Numerical Simulation on Steel Plate Girders With Deep Section
6 th International Conference on Advances in Experimental Structural Engineering 11 th International Workshop on Advanced Smart Materials and Smart Structures Technology August 12, 2015, University of
More informationCHARACTERIZING INFLUENCE OF LAMINATE CHARACTERISTICS ON ELASTIC PROPERTIES OF CROSS LAMINATED TIMBER
CHARACTERIZING INFLUENCE OF LAMINATE CHARACTERISTICS ON ELASTIC PROPERTIES OF CROSS LAMINATED TIMBER Jan Niederwestberg 1, Ying Hei Chui ABSTRACT: Properties of CLT panels are influenced by the properties
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationThe stiffness of plates
The stiffness of plates 1. Introduction The word plate is a collective term for elements in which forces can be transferred in two directions. Floors, walls, bridge slabs and laminates are all plates.
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationStrength of Materials (15CV 32)
Strength of Materials (15CV 32) Module 1 : Simple Stresses and Strains Dr. H. Ananthan, Professor, VVIET,MYSURU 8/21/2017 Introduction, Definition and concept and of stress and strain. Hooke s law, StressStrain
More informationKINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK. Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV
KINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV UNIT I STRESS, STRAIN DEFORMATION OF SOLIDS PART A (2 MARKS)
More informationQUESTION BANK DEPARTMENT: CIVIL SEMESTER: III SUBJECT CODE: CE2201 SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A
DEPARTMENT: CIVIL SUBJECT CODE: CE2201 QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationSTRESS, STRAIN AND DEFORMATION OF SOLIDS
VELAMMAL COLLEGE OF ENGINEERING AND TECHNOLOGY, MADURAI 625009 DEPARTMENT OF CIVIL ENGINEERING CE8301 STRENGTH OF MATERIALS I 
More informationSERVICEABILITY LIMIT STATE DESIGN
CHAPTER 11 SERVICEABILITY LIMIT STATE DESIGN Article 49. Cracking Limit State 49.1 General considerations In the case of verifications relating to Cracking Limit State, the effects of actions comprise
More informationDirect and Shear Stress
Direct and Shear Stress 1 Direct & Shear Stress When a body is pulled by a tensile force or crushed by a compressive force, the loading is said to be direct. Direct stresses are also found to arise when
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More informationPurpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on Exam 3.
ES230 STRENGTH OF MTERILS Exam 3 Study Guide Exam 3: Wednesday, March 8 th inclass Updated 3/3/17 Purpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationMechanics of Biomaterials
Mechanics of Biomaterials Lecture 7 Presented by Andrian Sue AMME498/998 Semester, 206 The University of Sydney Slide Mechanics Models The University of Sydney Slide 2 Last Week Using motion to find forces
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationESE TOPICWISE OBJECTIVE SOLVED PAPER I
C I V I L E N G I N E E R I N G ESE TOPICWISE OBJECTIVE SOLVED PAPER I FROM 1995018 UPSC Engineering Services Eamination, State Engineering Service Eamination & Public Sector Eamination. Regd. office
More informationAERO 214. Lab II. Measurement of elastic moduli using bending of beams and torsion of bars
AERO 214 Lab II. Measurement of elastic moduli using bending of beams and torsion of bars BENDING EXPERIMENT Introduction Flexural properties of materials are of interest to engineers in many different
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationPART A. CONSTITUTIVE EQUATIONS OF MATERIALS
Preface... xix Acknowledgements... xxix PART A. CONSTITUTIVE EQUATIONS OF MATERIALS.... 1 Chapter 1. Elements of Anisotropic Elasticity and Complements on Previsional Calculations... 3 Yvon CHEVALIER 1.1.
More informationQUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS
QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State Hooke s law. 3. Define modular ratio,
More informationRELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer
RELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer and Robert J. Ross Supervisory Research Engineer USDA Forest Service Forest Products
More informationSimultaneous measurement of critical current, stress, strain and lattice distortions in high temperature superconductors
Simultaneous measurement of critical current, stress, strain and lattice distortions in high temperature superconductors C. Scheuerlein 1, R. Bjoerstad 1, A. Grether 1, M. Rikel 2, J. Hudspeth 3, M. Sugano
More informationConstitutive model for quasistatic deformation of metallic sandwich cores
INTERNATIONAL JOURNAL FOR NUMERICAL METHODS IN ENGINEERING Int. J. Numer. Meth. Engng 2004; 61:2205 2238 Published online 18 October 2004 in Wiley InterScience (www.interscience.wiley.com). DOI: 10.1002/nme.1142
More informationCharacterizations of Aluminum Alloy Sheet Materials Numisheet 2005
Characterizations of Aluminum Alloy Sheet Materials Numisheet 25 John C. Brem, Frederic Barlat, Robert E. Dick, and JeongWhan Yoon Alcoa Technical Center, PA, 15691, USA Abstract. This report reproduces
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationConstitutive Equations
Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module
More informationCOURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5
COURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5 TIME SCHEDULE MODULE TOPICS PERIODS 1 Simple stresses
More informationMATERIAL PROPERTIES. Material Properties Must Be Evaluated By Laboratory or Field Tests 1.1 INTRODUCTION 1.2 ANISOTROPIC MATERIALS
. MARIAL PROPRIS Material Properties Must Be valuated By Laboratory or Field ests. INRODUCION he fundamental equations of structural mechanics can be placed in three categories[]. First, the stressstrain
More informationHOT MIX ASPHALT CYCLIC TORQUE TESTS FOR VISCOELASTIC BULK SHEAR BEHAVIOUR
1 1 1 1 1 1 1 1 0 1 0 1 0 HOT MIX ASPHALT CYCLIC TORQUE TESTS FOR VISCOELASTIC BULK SHEAR BEHAVIOUR Petit Christophe 1, Allou Fatima 1, Millien Anne 1, Fakhari Terhani Fateh, Dopeux Jérome 1 ( 1 Laboratoire
More information